Surface Relief Due to Bainite Transformation at 473 K (200 °C)
- 1.1k Downloads
Extremely thin plates of bainitic ferrite can now routinely be induced in steels by heat–treatment at low homologous temperatures. Given the atomic mechanism by which the transformation occurs, morphology should be dominated by the minimization of strain energy due to the displacements necessary to accomplish the change in crystal structure when austenite decomposes into bainite. Experiments were conducted using atomic force microscopy in an attempt to characterize these displacements, with a surprising outcome that the shear strain is much larger than associated with conventional, coarser bainitic structures. It appears that this might explain why the plates of bainitic ferrite tend to be slender in this new class of nanostructured alloys.
KeywordsAustenite Shear Strain Cementite Bainite Bainitic Ferrite
Novel steels containing high concentrations of carbon and silicon were developed by Caballero and co-workers,[1, 2, 3] and the international activity in this developing field was recently reviewed; the most recent publication is by Hu and Wu. The steels are a development of carbide-free bainitic alloys, in which silicon is used to suppress the precipitation of cementite from the residual austenite during the course of bainite transformation.[6,7] A most significant feature of the alloy design is that the bainite is able to form at unconventionally low temperatures, resulting in a structure of incredibly fine plates of bainitic ferrite in a matrix of carbon-enriched retained austenite, resulting in a dramatic increase in hardness and strength while at the same time achieving reasonable fracture toughness and ductility. The material is now commercially available, and the manufacturing process established to a point where many hundreds of tonnes have been produced successfully.
The very fine structure offers an intriguing opportunity to explore the fundamental characteristics of bainite that form at temperatures as low as a quarter of the homologous temperature, where the diffusion distance of atoms on substitutional sites is negligibly small over the time scale of the transformation. A number of revealing experiments were reported using techniques such as the atom probe and in-situ measurements using high-energy X-ray sources.[9, 10, 11, 12, 13]
The plates of bainite that form at the low temperatures are some 20 to 40 nm in thickness; their shape deformations have yet to be characterized and may hold a clue to explaining why they are so thin. Optical interference techniques, which have been used successfully to look at the surface relief due to coarse plates of martensite, cannot be applied even to ordinary bainite, because their thickness, typically 0.2 μm, is below the wavelength of the light, so that any relief observed is an average due both to the bainite plates and intervening phases such as cementite and austenite. Sandvik resolved this issue by looking at the displacement of austenite twin boundaries by plates of bainitic ferrite using transmission electron microscopy and reported a shear strain associated with an individual plate to be 0.22. Swallow and Bhadeshia used atomic force microscopy to determine the shear strain to be about 0.26; theory predicts values in the range 0.22 to 0.28.
Observed Values for Invariant–Plane Strain for a Variety of Transformations
2 Experimental procedures
Samples were machined in the form of square-sectioned 4 mm × 4 mm × 30 mm rods, from an alloy of composition Fe-0.79C-1.59Si-1.94Mn-1.33Cr-0.3Mo-0.11V wt pct. They were then metallographically polished on all their surfaces to 1 μm, cleaned with high-purity ethanol, and sealed in partially evacuated quartz tubes flushed with argon in order to conduct the austenitization and isothermal transformation heat treatments. All of these measures help reduce contamination and oxidation of the polished surface, but to further reduce surface deterioration, titanium powder was added to the tubes in order to getter any remaining traces of oxygen. Austenitization was carried out for 15 minutes at 1473 K (1200 °C) before isothermal transformation at 473 K (200 °C) for 7 days, which is sufficient time that the microstructure can be expected to be a mixture of bainite and austenite based on previous results.
A SPA-300 (Seiko Instruments Inc., Chiba, Japan) atomic force microscope was operated in contact mode with a 20-μm scanner table and a force reference of 1.95 nN. Images were acquired with 512 × 512 pixel resolution; the maximum scan speed used for imaging was 1 Hz, and this was reduced in order to prevent artefacts due to excessive “jumping” of the tip caused by scanning over the surface. The voltage sensitivity for the vertical dimension (nm mV−1) was calculated automatically based on the dimensions and resonant frequency of the cantilever, which were supplied by the manufacturer who measured the dimensions of each tip. The quoted accuracy of the frequency is 10 pct, resulting in 10 pct error in the measurement of the vertical dimension. Horizontal dimensions were not calibrated; however, it is reasonable to believe that the errors from surface artefacts and vertical calibration will be much larger than the error in measuring the horizontal dimensions.
3 Results and Discussion
The true shear s due to an individual plate, and indeed the thickness of the plate, can only be measured directly if the habit plane of the plate is normal to the plane of observation. The plates, however, generally will be inclined to the surface so that the measurement represents an apparent shear component s A , which was determined using the gradient of the scan across the plate, s A = height/width. There is a further complication that the austenite adjacent to the bainite plate may relax by plastic deformation. The side corresponding to the bainitic ferrite can be identified from the shape of the lenticular plate in the context of adjacent plates (Figure 5). Furthermore, the angle of shear of adjacent plates should be similar, because they should have similar crystallographic orientation within a bainite sheaf. Plastic accommodation in the austenite involves multiple slip systems resulting in intense dislocation tangles and irregular relief.
It should be noted that in the experiments reported here, the observation plane and specimen surface were both horizontal. Because of the different magnifications of the vertical and horizontal scales, simply looking at the 3-D representations and the topographic line scans can give an exaggerated view of the magnitude of the features, as demonstrated by comparing Figures 3(a) and (b). If the shear component is around 0.25 to 0.28, the features expected due to shearing should be 3.5 to 4 times wider than they are high; it may be more useful to interpretation of the data to plot the data with a 1:1 ratio between the scales of height and horizontal displacement, as demonstrated in Figures 4 and 5.
Plotting the observed values against the plate width shows the tendency implied by these equations (Figure 6). If all the plates are of equal true thickness, then the plates, which are seen as wide in their two-dimensional projections on the plane of observation, have relatively shallow inclination to that plane and hence a smaller apparent shear. This is precisely the trend observed in Figure 6; however, a corrected shear could not be reliably calculated, presumably because there is also a spread in the true plate widths. For this reason, the largest shears measured have to be used as the best indication as to the value of the shear component.
It is emphasized that these calculations assume that each plate measured makes a substantial intersection with the free surface. The plates have a lenticular morphology,[20,21] so if only the periphery of a deeply located plate intersects the free surface, then the apparent width will be smaller. This, together with the fact that the orientation of the displacement vector of the shape deformation can vary relative to the free surface, could explain why different values of apparent shear are observed for the same apparent width in Figure 6. Neither of these observations detract from the fact that the maximum observed value of the shear will be closer to the actual shear.
A value of ≈0.46 was determined for the shear component of the displacements due to individual plates of bainitic ferrite transformed at 473 K (200 °C). This is larger than previously reported using the same experimental technique but for bainite generated by transformation at a higher temperature. The large shear is consistent with the slender character of the bainitic ferrite plates that form at low homologous temperatures and is not unprecedented in the context of solid-state phase transformations in steels. It is speculated that different modes of lattice invariant deformation might operate when the transformation occurs in the austenite that is strengthened by the large carbon concentration of the alloy studied and the lower temperature at which transformation was induced.
The authors are grateful to the Engineering and Physical Sciences Research Council and to Corus plc. (now Tata Steel) for their support of this work.
- 5.F. Hu and K. Wu: Adv. Mater. Res., 2011, vols. 146–147, pp. 1843–48.Google Scholar
- 6.H.K.D.H. Bhadeshia and D.V. Edmonds: Met. Sci., 1983, vol. 17, pp. 411–19.Google Scholar
- 8.Patent No. GB2462197, Intellectual Property Office, London, 2010.Google Scholar
- 13.F.G. Caballero, M.K. Miller, A.J. Clarke, and C. Garcia-Mateo: Acta Mater., 2010, vol. 63, pp. 442–45.Google Scholar
- 14.B.P.J. Sandvik and H.P. Nevalainen: Met. Technol., 1981, vol. 8, pp. 213–20.Google Scholar
- 15.E. Swallow and H.K.D.H. Bhadeshia: Mater. Sci. Technol., 1996, vol. 12, pp. 121–25.Google Scholar
- 17.B.J.P. Sandvik: Metall. Trans. A, 1982, vol. 13A, pp. 777–87.Google Scholar
- 19.H.K.D.H. Bhadeshia and D.V. Edmonds: Metall. Trans. A, 1979, vol. 10A, pp. 895–907.Google Scholar
- 20.G.R. Srinivasan and C.M. Wayman: Trans. TMS-AIME, 1968, vol. 242, pp. 78–81.Google Scholar